IOSR Journal of Applied Physics (IOSR-JAP) e-ISSN: 2278-4861. Volume 3, Issue 3 (Mar. - Apr. 2013), PP 19-23 www.iosrjournals.org

Correlation between ground state properties and plasmon energy of ternary chalcopyrite semiconductors. S.K.Gorai1 , Parmanand Mahto2 1

2

(Department of physics,Tata College Chaibasa/ KolhanUniversity, India) (Department of physics,Vinoba Bhave University,Hazaribagh-825301,India)

Abstract : A simple relation between microhardness , plasmon energy, bulk modulus, electronic polarisability are given for ternary chalcopyrite semiconductors. Microhardness has been estimated from plasmon energy by proposing a linear relation between them.From microhardness ,bulk modulus has been estimated and refractive index is estimated from bulk modulus and subsequently polarisability has been estimated. The results are in excellent agreement with the available experimental data and earlier researchers. Keywords –Plasmon energy,Bulkmodulus,Microhardness,Chalcopyrites,Polarisability . I.

INTRODUCTION

The ternary chalcopyrite semiconductors are technologically important group of semiconductors and have been studied extensively in last three decades,especially for their linear and nonlinear optical properties[12].The broad range of optical band gap and carrier mobilities offered by the binary ABC 2 semiconductors as well as their ability to form various solid solution and to accommodate different dopants has led to their emergence as technologically significant device materials, including application in photovoltaic solar cells, light emmiting diodes, infrared detectors etc. Although different methods of materials preparation for these chalcopyrites (I-III-VI2 and II-IV-V2) compounds have been suggested [3-6].These semiconductors crystallize in the chalcopyrite structure which is deduced from that of zinc blende by the replacement of cationic sublattice by two different atomic species.This induces the doubling of unit cell in a direction ,which is conventionally called c and a tetragonal distortion.This distortion is characterized by the parameter η=c/2a,where a and c are lattice parameters and by the anion displacement u=0.25+(d 2 A-C+d2 B-C)/a2 from its position in the cubic cell, where d A-C and d B-C are the cation-anion distances. Because of the added structural (η,u) and chemical (d A-C and d B-C ) degrees of freedom relative to their binary analogue, the ternary semiconductors exhibit a wide range of interesting physical chemical properties. The knowledge of many of the physicochemical properties that are essential for designing appropriate conditions for the growth of bulk single crystals and of high quality epitaxial layers is still inadequate.In this regard some mechanical properties such as microhardness, bulk modulus and optical properties such as polarisability have been studied.There have been various experimental and theoretical calculations based on empirical relations which have become an essential part of material research.Empirical formulae are mostly found to be simple, easy to use and gave a better value for physical parameters such as energy gap,dielectric constants,crystal ionicity, bondlength of semiconductors, empirical radii, electronegativity,ionicity and plasmon energy.The basic properties of molecules and solids are explained with the character of chemical bond. In chemical bond it is the valence electrons that takes part. These electrons reside in the outermost shell of the atom. Verma and Bhardwaj[7-8],Verma and Sharma[9-11] have recently calculated the electronic,mechanical and optical properties of semiconductors and insulators with the help of ionic charge theory of solids .In this paper we have calculated microhardness, bulk modulus, polarisability of AIBIIICVI2 and AIIBIVCV2 ternary chalcopyrites which are in excellent agreement with the previous estimation [12,13].A fairly good agreement has been obtained between them.

II.

THEORY, RESULTS AND CALCULATION

Microhardness is not an intrinsic material property since it represents the resistance of material to plastic deformation and it involves the nature of dislocation motion.An empirical relation between microhardness (H) and bonding parameters like valency of the atom in a crystal ,melting point and ionicity have been developed for ANB 8-N tetrahedral semiconductors and later on extended to A N-1B N+1C2 8-N (N=2,3) semiconductors. Ternary chalcopyrites of general compositions AIBIIIC2VI and AIIBIVC2 V can be considered as similar [15-17] to those of AIIBVI and AIIIBV binary tetrahedral semiconductors.According to Samanta et al.[18] microhardness (H) of AIBIIIC2VI and AIIBIVC2 V semiconductors may be expressed as

H = HB (

e e T f B 1 1 ) ( )1/2( 2 ) ( a 2 c ) (1- i ) ( m ) B V P T Fi d e

(1)

www.iosrjournals.org

19 | Page

Correlation between ground state properties and plasmon energy of ternary chalcopyrite where H B is a numerical constants with the unit of 10-14 kg. The term(

B V ) may be said to measure the V

availability of states for electron transfer where B denotes the limiting number of band states per metal atom of interacting set of atoms (e.g. B =8 for sp and 12 for sd bands), V is the number of valence electron per atom contributing to bonding, P is the mean periodicity of atom , d is the effective nearest neighbour distance ea and ec are valence numbers of anion and cation and e is the valence of pure covalent crystals f i is the mean value of ionicity of A-C and B-C bonds in ternary chalcopyrites. Fi =0.785 is the critical ionicity as defined as dielectric theory of Phillip[15] and Van Vechten [16] which separates four fold and six fold coordination scheme.Since equation(1) depends on the number of valence electrons which changes when a metal forms a compounds. These valence electrons when collectively oscillate in a solid is known as plasma oscillation in a solid. These oscillations in which all the valence or conduction electrons participate are a consequence both of inertia of the electrons and of their repulsive coulomb interaction. Such plasma oscillation in a solid can be excited in the electron gas either by fast energetic bombarding electrons [19,20] or during X-ray and Auger electron transitions[21,22].A plasmon is the quantum of elementary excitations associated with high frequency collective motion [23].Plasmon are studied by means of electron energy loss spectroscopy (EELS) and have been reported in recent years [24-28].Therefore we thought it would be of interest to propose an empirical relation between microhardness and plasmon energy of ternary chalcopyrites . We are of the view that the microhardness (H) of AIBIIIC2VI and AIIBIVC2 V semiconductors can be estimated using plasmon energy by the following relation as H=C( p ) –D (2) where C and D are constants,The values of C and D be 20.333,130.86 for A IBIIIC2VI and 271.64,3560.6 for AIIBIVC2 V semiconductors.The plasmon energy of ternary chalcopyrites is given by

p =

4Ne 2 m

(3)

where N is the valence electron density, e is the charge and m is the mass of the electron. In chalcopyrite compounds the effective number valence electrons of individual bond properties as

N

e

=

where

n e vb

(4)

ne =

z z N N

(5)

ne is the number of valence electrons of atom and .

N and N are the co-ordination number of

atoms and v b is the bond volume. The bond volume is

vb =4

3 d

(6)

3 3

for chalcopyrite structure where d is the mean value bond length of A-C and B-C bond present in these ternary chalcopyrites. The plasmon energy can be written as

p =28.8

Z M

(eV)

(7)

where Z is the effective number of valence electrons taking part in plasma oscillations , is the specific gravity and M is the molecular weight, p is the mean value of plasmon energy of individual bond length

p =( p

AC

+ p

B C

)/2 and d is the mean value of bond length.The bulk modulus defines its resistance

to volume change when compressed. Both experimental and theoretical result suggest that the bulkmodulus is a critical single material property to indicate hardness Neuman [13] has proposed the bulkmodulus microhardness relationship in AIIBIVC2 V chalcopyrite semiconductors by the following relation B=

CV0k H Tm

(8)

www.iosrjournals.org

20 | Page

Correlation between ground state properties and plasmon energy of ternary chalcopyrite where C and k are adjustable parameters.Cohen [30] and Lam et al [38]have investigated the bukmodulii and geometrical properties of diamond and ZB solids. Considering Phillips and VanVechten scheme [15,16 ] cohen has proposed the following empirical relation: B=(1971-220 ) d (9) where is an empirical parameter which accounts for the effect of ionicity , =0,1,2 for IV,III-V and II-VI compounds respectively, d is the nearest neighbours distance in A0 and B in GPa. Lam et al [30] has deduced bulk modulii to lattice parameters within the local density formalism and the pseudopotential as 3.5

3.5

4

B=1971 d -408 ( Z )2 d (10) where Z =1 and 2 for III-V and II-VI semiconductors. The modification of cohens relation (7) given by Grima and Gallardo [33] may be expressed in terms of average nearest neighbour distance and electronic susceptibilities of different bond by the following relation B= (1971-220 ) d

3.5

- | AC - BC | 2..5

(11)

where =0.72, d =( d AC + d BC )/2 and AC and BC are the electronic susceptibilities of the bond. Recently Reddy et al [39] have studied bulk modulli from microhardness as B=51.538 H n0.131 fi (10) (for AIBIIIC2VI ternary chalcopyrites) (12) B=33.057 H n0.131 fi (11) (for AIIBIVC2 V ternary chalcopyrites) (13) where H is the microhardness, n is the refractive index and fi is the ionicity of ternary chalcopyrite semiconductors. We propose a linear empirical relation between microhardness and bulk modulus of ternary chalcopyrite semiconductors.From the proposed relation we estimate bulk modulus from microhardness(calculated). The proposed relation as B=M(H)-N (14) where M and N are constants, their numerical values are M=0.0767,N=32.704 for II-IV-V2 compounds and M=0.8135,N=-85.703 for I-III-VI2 for compounds respectively. we propose another relation between bulk modulus and refractive index for evaluating the refractive index of A IBIIIC2VI and AIIBIVC2 V chalcopyrite respectively. The proposed equation as

n Ae KB

(15)

where n is the refractive index of ternary chalcopyrites and A,K are constants and their values are A =4.154,K=0.0028 for II-IV-V2 semiconductors and A=3.8263,K=-0.0052 for I-III-VI2 semiconductors respectively subsequently polarisability is estimated using Claussius –Mossotti equation as

n2 1 M ]x =0.395x10 [ 2 d n 2 -24

where

cm3

(16)

is the electronic polarisability, M and d are molecular weight and density of the chalcopyrites.

III.

Conclusion

We have estimated the microhardness of AIBIIIC2VI and AIIBIVC2 V semiconductors using plasmon energy of chalcopyrite semiconductors. From microhardness we estimate bulk modulus of semiconductors and subsequently polarisability is estimated from calculated values bulk modulus using claussius –Mossotti equation. The estimated values of polarisability of ternary chalcopyrites are given in table 3 and 4 for the comparison with other researchers. The plasmon energy is a key parameter for estimating optical and mechanical properties of the compounds concerned. We find that plasmon energy has a linear relation with the experimental values of microhardness and microhardness (calculated) has a linear relation with experimental value of bulk modulus. The estimated values of bulkmodulus and Microhardness of ternary chalcopyrites and their experimental values are given in table 1 and table 2 for the comparison. It also appears that our calculated values agree well with the experimental ones. Amongst the AIBIIIC2VI and AIIBIVC2 V compounds the former group materials posseses greater value H than the latter because of more covalent character of the former. On comparing the bulk modulus amongst it is seen that they all decrease for sulphide to selenide to telluride in case of Cu-III-VI2 compounds and the same features follows for Ag compounds.

www.iosrjournals.org

21 | Page

Correlation between ground state properties and plasmon energy of ternary chalcopyrite REFERENCES [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32] [33] [34] [35] [36] [37] [38] [39]

H Metzner,U Reislöhner ,J Cieslak,W Witthuhn , T Hahs T and Kraüßlichn, J Thin solid film, 13 (2002) 403. R W Birkmire and E Eser , Ann Rev mater Sci, 27 (1997) 625. J L Shay and J H Wernick, Ternary chalcopyrite semiconductors Growth, electronic properties and applications (Pergamon Press, New York) 1975. A Chahed ,O Benhelas ,H Rozale,S Laksoni and N Abboeni , Phys Status solidi (b), 244 (2007) 629. L Garbato and A Rucci , Chem Phys Lett, 61 (1979) 542. L K Samanta, D K Ghosh and G C Bhar , J Chem Phys, 79 (1983) 361. A S Verma and S R Bhardwaj , J Phys condens Matter, 18 (2006). A S Verma and S R Bhardwaj , Phys. Status solidi (b), 243 (2006) 4025. A S Verma and S R Bhardwaj ,, Phys script, 76 (2007) 22. A S Verma and D Sharma , Phys status solidi (b), 245 (2008) 678. A S Verma and A Kumar and S R Bhardwaj , Phys status solidi (b), 245 (2008) 1520. B F Levine , [a] Phys. Rev. B 7, (1973) 259; [b] J Chem phys, 59 (1973) 1463. H Neumann , [a] Crystal Res Technol 23, (1988) 97 [b] H Neumann Crystal Res Technol 24, (1989) 815. L Garbato L and A Rucci , Philo Mag, 35 (1977) 1681, 35 (1977) 1685. J C Phillip , Rey Mod Phys, (1970) 317. J A Van Vechten , Phys Rev, 182 (1969) 891. D S Chemla , Phys Rev letter, 26 (197) 1441. K L Samanta , and S Chatterjee , Phys Status sol (b) 182 (1994) K 85. D Pines , Solid state physics 1st (edn.) F Seitz and D Turnbell (Academic Press NY), 367 (1955). D Pines , Rev Mod Phys, 28 (1956) 184. R Ferrel , Rev Mod Phys, 28 (1956) 308. K S Srivastava,R L Srivastava ,O K Hansh and Y Kumar, J phys chem solids, 40 (1979) 489. D Pines, elementary excitation in solids (Benyamiior NY) 8 (1964). http://www.nims.go.jp/aperiodie/hrtem/recent/eels. Y Ohno , Phys Rev B, 46 (1992) B 46. S Narain, Phys status solidi (b), 182 (1994) 273. http://eprints gla.ac.vk/4716. J Robio and M Armientn, J Geo chem Explor, 68(2006) 167-181. K Widder , M Knupfer, O Knauff and J Frink , Phys Rev B, 56 10 (1997) 154. M L Cohen , Phys Rev B, 32 (1985) 7988. S A Borshchevskii , N A Goryunova , F P Kesamanly and D N asdedov , Phys Status Solidi, 21 (1967) 9. H Neumam , Phys Status Solidi (b), 182 (1986) K 121. P Grima Gallardo Phys Status Solidi (b), 182 (1994) K 67. R R Reddy , Y Nazeer Ahammed ,K Rama Gopal ,TVR Rao ,P Abdul Azeem and P Mallikarjuna Reddy , Optical Materials, 14 (1983) 361. R R Reddy , M Ravi Kumar and TVR Rao , Infrared Physics, 34 (1993) 95. V P Gupta and V K Srivastav , J Phys. Chem Solids, 42 (1981) 1079. V Kumar, G M Prasad and D Chandra Phys Status Solidi (b),186 (1994) K-454. P K Lam , M L Cohen and G Martinez , Phys Rev B, 35 (1987) 9190. R R Reddy , Y Nazeer Ahammed , K Ramagopal,D V Raghuram , Indian J pure Appl Phys, 37 (1999) 25.

Table 1 Plasmon energy, microhardness, bulk moduls of II-IV-V2 ternary chalcopyrites

p ZnSiP2 ZnSiAs2 ZnGeP2 ZnGeAs2 ZnGeP2 ZnGeAs2 ZnSnP2 ZnSnAs2 CdSiP2 CdSiAs2 CdGeP2 CdGeAs2 AgInTe2 CdSnAs2

H(Kg/mm2)

(eV)

Mol. Wt. (g)

Density (g/cm3 )

17.015 16.085 16.638 15.663 16.638 15.663 15.15 14.825 16.194 15.35 15.517 14.898 13.037 14.092

155.4 242.2 1.99.9 248.8 1.99.9 248.8 246 333.9 202.43 290.34 246.94 334.83 447.89 380.93

3.39 4.7 4.179 5.32 4.179 5.32 3.165 5.35 4 5.154 4.48 5.6 6.12 5.72

This work [eqn.(2)] 1061.35 808.72 958.94 694.09 958.94 694.09 663.40 466.46 838.33 609.07 654.43 486.29 134.22 267.35

B(GPa)

expt. [3,31]

Reported [5,18]

This work [eqn.(14)]

1100 920 980 680 980 680 455 744

1065, 900 890, 820 770, 635 680,630 770, 635 680,630 500,530 445,430 765,730 640,615 515,470 490,470 98,116 315,310

114.10 94.733 106.25 85.94 106.25 85.94 83.58 68.48 97.00 79.41 82.89 70.00 23.48 53.20

565 470 188 335

www.iosrjournals.org

expt. [32]

97

70

Reported [13a,33] 120 93 108 86 108 86 84 67 97 77 86 70 28 55

22 | Page

Correlation between ground state properties and plasmon energy of ternary chalcopyrite

Table 2 Plasmon energy, microhardness, bulk modulus of I-III-VI2 ternary chalcopyrites Compounds

CuAlS2 CuAlSe 2 CuAlTe2 CuGaS 2 CuGaSe 2 CuGaTe2 CuInS2 CuInSe2 CuInTe2 AgAlSe2 AgAlTe2 AgGaS2 AgGaSe2 AgGaTe 2 AgInSe2

p (eV)

Mol. Wt. (g)

Density (g/cm3 )

17.25 15.845 14.53 12.278 15.918 14.305 16.123 15.09 13.664 15.16 14.501 16.098 15.199 13.621 14.233

154.65 248.45 345.73 197.39 291.19 388.47 242.44 336.29 433.57 293.77 390.05 241.71 335.51 432.79 380.61

3.47 4.7 5.5 4.35 5.56 5.99 4.75 5.77 6.1 5.07 6.18 4.72 5.84 6.05 5.81

H(Kg/mm2) This work [eqn.(2)] 219.88 191.31 164.57 220.45 192.80 160.00 196.96 175.96 146.97 177.38 163.98 196.46 178.18 146.09 158.53

expt. [3,31] 210 182 197 180 185 152 160 149 150 127

B(GPa) Reported [5,18] 261,250 228,226 210,225 245,230 210,197 185,240 140,140 141,160 140,166 135,176 142,167 130,175 124 142,166 82,102

This work [eqn.(14)] 93.17 69.93 48.18 93.63 71.14 44.45 74.53 57.44 33.85 58.60 47.70 74.11 59.24 33.14 43.26

expt. [32]

Reported [13a,33] 94 69 45 93 68 43 71 54 36 55 36 70 53 35 42

94,96 71 44 62

Table 3. Electronic polarisability of II-VI-V2 ternary chalcopyrites. Compounds

p (eV)

ZnSiP2 ZnSiAs2 ZnGeP2 ZnGeAs2 ZnSnP 2 ZnSnAs2 CdSiP2 CdSiAs2 CdGeP 2 CdGeAs2 CdSnAs2

17.015 16.085 16.638 15.663 15.55 14.825 16.194 15.35 15.517 14.898 14.092

Electronic polarisability, Present Study (Eq.10) 13.21 15.32 13.97 14.09 23.50 18.64 15.00 17.14 16.68 18.43 20.97

10 24 (cm )

[Ref. 34] 12.27 15.04 13.54 16.82 14.54 19.10 13.58 16.05 18.43 21.33

3

Known [Ref. 35] 12.45 18.12 14.24 20.52 16.36 23.84 14.34 13.16 15.95 23.16 26.68

[Ref. 36,37] 10.70 12.89 11.28 12.62 13.80 14.99 12.29 12.88 12.15 17.32

Table 4. Electronic polarisability of I-III-VI2 ternary chalcopyrites. Compounds

p

CuAlS2 CuAlSe2 CuAlTe2 CuGaS2 CuGaSe2 CuGaTe2 CuInS2 CuInSe2 CuInTe2 AgAlSe2 AgAlTe2 AgGaS2 AgGaSe2 AgGaTe2 AgInS2 AgInSe2 AgInTe2

17.25 15.845 14.53 12.278 15.918 14.305 16.123 15.09 13.664 15.16 14.501 16.098 15.199 13.621 15.209 14.233 13.037

(eV)

Electronic polarisability, Present Study (Eq.10) 10.61 13.97 17.97 10.78 13.78 18.76 13.24 16.15 21.22 15.93 18.07 13.31 15.82 21.40 15.78 19.02 22.46

[Ref. 34] 10.82 13.76 19.10 12.06 15.27 19.7 13.29 16.42 22.63 13.68 16.07 14.43 16.57 21.73 14.45 20.08 24.08

www.iosrjournals.org

10 24 (cm ) 3

Known [Ref. 35] 6.73 10.09 17.17 7.25 10.91 19.20 8.43 12.47 20.86 11.31 19.35 8.22 12.13 20.79 9.04 13.51 13.23

[Ref. 36,37] 6.62 9.02 7.37 7.61 10.29 11.74 10.59 12.73 15.29 10.42 12.06 8.46 11.35 13.17 10.91 14.69 16.88

23 | Page

Read more

Similar to

Popular now

Just for you